Functionalized silicon quantum dots by N vinylcarbazole ...pom.henu.edu.cn ›...
Embed Size (px)
Transcript of Functionalized silicon quantum dots by N vinylcarbazole ...pom.henu.edu.cn ›...
Functionalized silicon quantum dots by N- vinylcarbazole: synthesis and spectroscopic properties
Jianwei Ji1,† Email: email@example.com
Guan Wang1,† Email: firstname.lastname@example.org
Xiaozeng You1* * Corresponding author Email: email@example.com
Xiangxing Xu1* * Corresponding author Email: firstname.lastname@example.org
1 State Key Laboratory of Coordination Chemistry, Nanjing National Laboratory of Microstructures, School of Chemistry and Chemical Engineering, Nanjing University, Nanjing 210093, People's Republic of China
† Equal contributors.
Silicon quantum dots (Si QDs) attract increasing interest nowadays due to their excellent optical and electronic properties. However, only a few optoelectronic organic molecules were reported as ligands of colloidal Si QDs. In this report, N-vinylcarbazole - a material widely used in the optoelectronics industry - was used for the modification of Si QDs as ligands. This hybrid nanomaterial exhibits different spectroscopic properties from either free ligands or Si QDs alone. Possible mechanisms were discussed. This type of new functional Si QDs may find application potentials in bioimaging, photovoltaic, or optoelectronic devices.
Silicon quantum dots, N-vinylcarbazole, Surface modification, Spectroscopic property
Silicon (Si) is one of the most important semiconductor materials for the electronics industry. The energy structure of bulk Si is indirect bandgap, which is greatly changed by the quantum confinement effect for small enough Si nanocrystals (NCs) called Si quantum dots (QDs), making Si QDs fluorescent with a tunable spectrum. Excellent spectroscopic properties, such as high quantum yield, broad absorption window, and narrow fluorescent wavelength, contribute to a rapid development in Si QD research . Nontoxicity to the environment and
the use of an economic source material are other two merits for the application of Si QDs in optoelectronics [2,3], solar energy conversion [4,5], biology [6-8], splitting water , etc. Si QDs can be prepared using a variety of techniques such as wet chemical reduction [10-18], metathesis reaction , disproportionation reaction [20,21], thermal annealing of Si-rich SiC , electrochemical etching , plasma synthesis or plasma-enhanced chemical vapor deposition (PECVD) [24-27], and high-temperature hydrogen reduction method [28-32]. Because Si QDs are chemically active, their surface should be passivated for further use. Molecules with alkyl chains and -CH3, -COOH, or -NH2 ends have been widely employed as surface ligands to enhance the stability of Si QDs [28-36]. These ligands help prevent the oxidation of silicon and enhance the dispersibility of Si QDs in organic or aqueous solution. In addition to the surface protection, optoelectronic functional molecules as ligands of Si QDs are attracting increasing interest in recent years for the crucial role of the ligands to the interfacial related process in optoelectronic or light-harvesting devices. Kryschi and co- workers showed that 3-vinylthiophene ligands may act as surface-bound antennae that mediate ultrafast electron transfer or excitation energy transfer across the Si QD interface via high-energy two-photon excitation [37,38]. They also reported that for 2- and 4- vinylpyridine-terminated Si QDs, ultrafast excitation relaxation dynamics involving decay and rise dynamics faster than 1 ps were ascribed to electronic excitation energy transfer from an initially photoexcited ligand state to Si QD conduction band states . Larsen and Kauzlarich and their co-workers investigated the transient dynamics of 3-aminopropenyl- terminated Si QDs . A formation and decay of a charge transfer excited state between the delocalized π electrons of the carbon linker and the Si core excitons were proposed to interpret one-photon excitation. Zuilhof et al. reported Si QDs functionalized with a red- emitting ruthenium complex to exhibit Förster resonance energy transfer (FRET) from Si QDs to the complex . The ligands on the Si surface may also induce optoelectronic interactions to other QDs such as CdSe QDs, e.g., Sudeep and Emrick found that hydrosilylation of Si QDs provides a corona of phosphine oxides that may serve as ligands for CdSe QDs . This surface functionalization of the Si QDs was proved a key to the photoluminescence quenching of CdSe QDs, as conventional (alkane-covered) Si QD samples give no evidence of such optoelectronic interactions. Recently, we reported 9- ethylanthracene-modified Si QDs showing dual emission peaks that originate from the Si QD core and the ligands . In this report, we demonstrate the synthesis and surface modification of Si QDs with N-ethylcarbazole, using hydrogen-terminated Si QDs and N- vinylcarbazole as the starting materials. Both anthracene and carbazole are fluorescent molecules and organic semiconductors. The main difference is that anthracene is an electron transport material while carbazole is a hole transport material. This difference is important for the structure design of optoelectronic or photovoltaic devices utilizing these Si QD-based hybrid materials. N-vinylcarbazole and its derivatives as a class of typical optoelectronic molecules show abundant attractive properties and can be applied in dye, optics, electronics, and biology [44-48]. N-vinylcarbazole is also the monomer precursor of poly(N- vinylcarbazole) (PVK) polymer which is widely used as a hole transport or electroluminescent material in organic optoelectronic devices [49-51]. The N-ethylcarbazole- modified Si QDs (referred to as ‘N-ec-Si QDs’ for short) exhibit photoluminescence quite different from freestanding N-vinylcarbazole- or hydrogen-modified Si QDs. This hybrid nanomaterial was characterized and investigated by powder X-ray diffraction (XRD), transmission electron microscopy (TEM), Fourier transform infrared spectroscopy (FTIR), photoluminescence (PL), and PL lifetime measurement.
Materials and equipment
N-vinylcarbazole (98%), HSiCl3 (99%), and mesitylene (97%) were purchased from Aladdin Reagent Co., Ltd. (Shanghai, China). Analytical-grade ethanol (99.5%) and hydrofluoric acid (40% aqueous solution) were received from Sinopharm Chemical Reagent Co., Ltd. (SCRC; Shanghai, China). All reagents were used as purchased without further purification. The XRD spectrum was performed on a Bruker D8 Advance instrument (Bruker AXS GmbH, Karlsruhe, Germany) with Cu Kα radiation (λ = 1.5418 Å). TEM images were obtained on a JEM-2100 transmission electron microscope with an acceleration voltage of 200 kV (JEOL, Ltd., Akishima, Tokyo, Japan). The FTIR spectra were measured by a Bruker VECTOR 22 spectrometer (Bruker, Germany) with KBr pellets. The PL and excitation spectra were collected by a Hitachi F-4600 fluorescence spectrophotometer (Hitachi, Ltd., Chiyoda-ku, Japan). The UV-vis absorption spectra were measured by a Shimadzu UV-2700 UV-vis spectrophotometer (Shimadzu Corporation, Kyoto, Japan). The PL lifetime was obtained on a Zolix Omni-λ 300 fluorescence spectrophotometer (Zolix Instruments Co., Ltd., Beijing, China).
Synthesis of hydrogen-terminated Si QDs
Si QDs were synthesized by reduction of (HSiO1.5)n powder with hydrogen [28,29]. Typically, 5 mL of HSiCl3 (49.5 mmol) was added to a three-neck flask equipped with a mechanical stir bar, cooled to −78°C in an ethanol bath, and kept for 10 min, using standard Schlenk techniques with N2 protection. With the injection of 20 mL H2O by a syringe, a white precipitate formed immediately. After 10 min, the white (HSiO1.5)n was collected by centrifugation, washed by distilled water, and dried in vacuum at 60°C. In the reduction step, (HSiO1.5)n (1.10 g) was placed in a corundum crucible and transferred to a tube furnace. The sample was heated to 1,150°C and maintained for 1.5 h with a heating rate of 5°C/min under a slightly reducing atmosphere containing 5% H2 and 95% Ar (≥99.999%). After cooling to room temperature, a light brown product of Si/SiO2 composite was collected. The Si/SiO2 composite (50 mg) was grinded with a mortar and pestle for 10 min. Then the powder was transferred to a Teflon container (20 mL) with a magnetic stir bar. A mixture of ethanol (1.5 mL) and hydrofluoric acid (40%, 2.5 mL) was added. The light brown mixture was stirred for 60 min to dissolve the SiO2. Finally, 5 mL mesitylene was added to extract the hydrogen- terminated Si QDs into the upper organic phase, forming a brown suspension (A), which was isolated for further surface modification.
Modification of Si QDs by functional organic molecules
N-vinylcarbazole (1 mmol) was dissolved in 15 mL mesitylene and loaded in a 50-mL three- neck flask equipped with a reflux condenser. Then 2 mL Si QDs (A) was injected by a syringe. The mixture was degassed by a vacuum pump for 10 min to remove any dissolved gases from the solution. Protected by N2, the solution was heated to 156°C and kept for 12 h. After cooling to room temperature, the resulting Si QDs were purified by vacuum distillation and then washed by ethanol to remove excess solvent and organic ligands. The as-prepared brown solid product was readily re-dispersed in mesitylene to give a yellow solution.
Results and discussion
The synthesis route of N-ec-Si QDs is summarized in Figure 1. The HSiCl3 hydrolysis product (HSiO1.5)n was reduced by H2 at 1,150°C for 1.5 h. In this step, the temperature and time are crucial in controlling the size of Si QDs. The higher the temperature and the longer the reduction time, the bigger the sizes of Si QDs. The following HF etching